LMucko/crystallography-open-database huggingface dataset:
Synthesis, structure and physical properties of layered semiconductors M Cu F Ch (M=Sr, Eu, Ch=S, Se)
Motomitsu, E.; Yanagi, H.; Kamiya, T.; Hirano, M.; Hosono, H.; Journal of Solid State Chemistry 179 (2006) 1668–1673; doi:

data_1528747
_publ_section_title
;
 Synthesis, structure and physical properties of layered semiconductors M
 Cu F Ch (M=Sr, Eu, Ch=S, Se)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1668
_journal_page_last               1673
_journal_volume                  179
_journal_year                    2006
_chemical_formula_sum            'Cu Eu F S'
_chemical_name_systematic        'Eu Cu F S'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.949
_cell_length_b                   3.949
_cell_length_c                   8.642
_cell_volume                     134.769
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Motomitsu_JSSCBI_2006_1157.cif
_cod_data_source_block           Cu1Eu1F1S1
_cod_original_cell_volume        134.7685
_cod_original_formula_sum        'Cu1 Eu1 F1 S1'
_cod_database_code               1528747
Synthesis, structure and physical properties of layered semiconductors M Cu F Ch (M=Sr, Eu, Ch=S, Se)
Motomitsu, E.; Yanagi, H.; Hosono, H.; Kamiya, T.; Hirano, M.; Journal of Solid State Chemistry 179 (2006) 1668–1673; doi:

data_1528748
_publ_section_title
;
 Synthesis, structure and physical properties of layered semiconductors M
 Cu F Ch (M=Sr, Eu, Ch=S, Se)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1668
_journal_page_last               1673
_journal_volume                  179
_journal_year                    2006
_chemical_formula_sum            'Cu F Se Sr'
_chemical_name_systematic        'Sr Cu F Se'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.063
_cell_length_b                   4.063
_cell_length_c                   8.842
_cell_volume                     145.963
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Motomitsu_JSSCBI_2006_1158.cif
_cod_data_source_block           Cu1F1Se1Sr1
_cod_original_cell_volume        145.9635
_cod_original_formula_sum        'Cu1 F1 Se1 Sr1'
_cod_database_code               1528748
Synthesis, structure and physical properties of layered semiconductors M Cu F Ch (M=Sr, Eu, Ch=S, Se)
Motomitsu, E.; Yanagi, H.; Kamiya, T.; Hosono, H.; Hirano, M.; Journal of Solid State Chemistry 179 (2006) 1668–1673; doi:

data_1528749
_publ_section_title
;
 Synthesis, structure and physical properties of layered semiconductors M
 Cu F Ch (M=Sr, Eu, Ch=S, Se)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1668
_journal_page_last               1673
_journal_volume                  179
_journal_year                    2006
_chemical_formula_sum            'Cu Eu F Se'
_chemical_name_systematic        'Eu Cu F Se'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.057
_cell_length_b                   4.057
_cell_length_c                   8.815
_cell_volume                     145.088
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Motomitsu_JSSCBI_2006_1159.cif
_cod_data_source_block           Cu1Eu1F1Se1
_cod_original_cell_volume        145.0883
_cod_original_formula_sum        'Cu1 Eu1 F1 Se1'
_cod_database_code               1528749
Cluster-Type Basic Lanthanide Iodides [M6(μ6-O)(μ3-OH)8(H2O)24]I8(H2O)8(M = Nd, Eu, Tb, Dy)
Mudring, Anja-Verena; Timofte, Tudor; Babai, Arash; Inorganic Chemistry 45 (2006) 5162–5166; doi:10.1021/ic051234s

data_4343879
_publ_section_title
;
 Cluster-Type Basic Lanthanide Iodides
 [M6(\m6-O)(\m3-OH)8(H2O)24]I8(H2O)8(M = Nd, Eu, Tb, Dy)
;
_journal_coden_ASTM              INOCAJ
_journal_issue                   13
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5162
_journal_page_last               5166
_journal_paper_doi               10.1021/ic051234s
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Dy6 H72 I8 O41'
_chemical_name_systematic        '(Dy6 O (O H)8 (H2 O)24) I8 (H2 O)8'
_space_group_IT_number           58
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.9634
_cell_length_b                   14.8613
_cell_length_c                   14.9188
_cell_volume                     2874.151
_cod_duplicate_entry             4331599
_cod_data_source_file            Mudring_INOCAJ_2006_1074.cif
_cod_data_source_block           H72Dy6I8O41
_cod_original_formula_sum        'H72 Dy6 I8 O41'
_cod_database_code               4343879
Cluster-Type Basic Lanthanide Iodides [M6(μ6-O)(μ3-OH)8(H2O)24]I8(H2O)8(M = Nd, Eu, Tb, Dy)
Mudring, Anja-Verena; Timofte, Tudor; Babai, Arash; Inorganic Chemistry 45 (2006) 5162–5166; doi:10.1021/ic051234s

data_4343880
_publ_section_title
;
 Cluster-Type Basic Lanthanide Iodides
 [M6(\m6-O)(\m3-OH)8(H2O)24]I8(H2O)8(M = Nd, Eu, Tb, Dy)
;
_journal_coden_ASTM              INOCAJ
_journal_issue                   13
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5162
_journal_page_last               5166
_journal_paper_doi               10.1021/ic051234s
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'H72 I8 O41 Tb6'
_chemical_name_systematic        '(Tb6 O (O H)8 (H2 O)24) I8 (H2 O)8'
_space_group_IT_number           58
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.9634
_cell_length_b                   14.8613
_cell_length_c                   14.9188
_cell_volume                     2874.151
_cod_duplicate_entry             4331605
_cod_data_source_file            Mudring_INOCAJ_2006_1075.cif
_cod_data_source_block           H72I8O41Tb6
_cod_database_code               4343880
Crystal structure elucidation of anhydrous Rb2 [Pt (C N)4] from x-ray powder diffraction data
Muehle, C.; Karpov, A.; Jansen, M.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 60 (2005) 1269–1272; doi:

data_7221495
_publ_section_title
;
 Crystal structure elucidation of anhydrous Rb2 [Pt (C N)4] from x-ray
 powder diffraction data
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1269
_journal_page_last               1272
_journal_volume                  60
_journal_year                    2005
_chemical_formula_sum            'C4 N4 Pt Rb2'
_chemical_name_systematic        'Rb2 (Pt (C N)4)'
_space_group_IT_number           74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.1432
_cell_length_b                   7.4382
_cell_length_c                   11.1896
_cell_volume                     927.454
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Muehle_ZNBSEN_2005_748.cif
_cod_data_source_block           C4N4Pt1Rb2
_cod_original_cell_volume        927.4539
_cod_original_formula_sum        'C4 N4 Pt1 Rb2'
_cod_database_code               7221495
La9 Rb Ir4 O24: A rubidium containing oxide with a new structure type
Mugavero, S.J.; Smith, M.D.; zur Loye, H.C.; Inorganic Chemistry 45 (2006) 946–948; doi:

data_4343881
_publ_section_title
;
 La9 Rb Ir4 O24: A rubidium containing oxide with a new structure type
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              946
_journal_page_last               948
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Ir4 La9 O24 Rb'
_chemical_name_systematic        'La9 Rb Ir4 O24'
_space_group_IT_number           87
_symmetry_space_group_name_Hall  '-I 4'
_symmetry_space_group_name_H-M   'I 4/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.7422
_cell_length_b                   7.7422
_cell_length_c                   17.7979
_cell_volume                     1066.836
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Mugavero_INOCAJ_2006_680.cif
_cod_data_source_block           Ir4La9O24Rb1
_cod_original_formula_sum        'Ir4 La9 O24 Rb1'
_cod_database_code               4343881
Neutron Structural Refinement of Cubic Orthotelluric Acid
Mullica, D.F.; Korp, J.D.; Mulligan, W.O.; Beall, G.W.; Bernal, I.; Acta Crystallographica B (24,1968-38,1982) 36 (1980) 2565–2570; doi:

data_2106569
_publ_section_title
;
 Neutron Structural Refinement of Cubic Orthotelluric Acid
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2565
_journal_page_last               2570
_journal_volume                  36
_journal_year                    1980
_chemical_formula_sum            'H6 O6 Te'
_chemical_name_systematic        'Te (O H)6'
_space_group_IT_number           210
_symmetry_space_group_name_Hall  'F 4d 2 3'
_symmetry_space_group_name_H-M   'F 41 3 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            32
_cell_length_a                   15.699
_cell_length_b                   15.699
_cell_length_c                   15.699
_cell_volume                     3869.154
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Mullica_ACBCAR_1980_62.cif
_cod_data_source_block           H6O6Te1
_cod_original_formula_sum        'H6 O6 Te1'
_cod_database_code               2106569
Refined crystal structure of lanthanum hexacyanoferrate(III) tetrahydrate
Mullica, D.F.; Milligan, W.O.; Garner, R.L.; Acta Crystallographica B (24,1968-38,1982) 36 (1980) 2561–2564; doi:

data_2106570
_publ_section_title
;
 Refined crystal structure of lanthanum hexacyanoferrate(III) tetrahydrate
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2561
_journal_page_last               2564
_journal_volume                  36
_journal_year                    1980
_chemical_formula_sum            'C6 H8 Fe La N6 O4'
_chemical_name_systematic        'La (Fe (C N)6) (H2 O)4'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   7.541
_cell_length_b                   7.541
_cell_length_c                   13.955
_cell_volume                     687.256
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Mullica_ACBCAR_1980_63.cif
_cod_data_source_block           C6H8Fe1La1N6O4
_cod_original_cell_volume        687.2557
_cod_original_formula_sum        'C6 H8 Fe1 La1 N6 O4'
_cod_database_code               2106570
Synthesis and study of the crystallographic and magnetic structure of Ho Fe Mn O3
Munoz, A.; Alonso, J.A.; Martinez-Lope, M.J.; Martinez, J.L.; European Journal of Inorganic Chemistry 2007 (2007) 1972–1979; doi:

data_4031256
_publ_section_title
;
 Synthesis and study of the crystallographic and magnetic structure of Ho
 Fe Mn O3
;
_journal_name_full               'European Journal of Inorganic Chemistry'
_journal_page_first              1972
_journal_page_last               1979
_journal_volume                  2007
_journal_year                    2007
_chemical_formula_sum            'Fe0.92 Ho Mn1.08 O4.74'
_chemical_name_systematic        'Ho Fe0.92 Mn1.08 O4.74'
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.2793
_cell_length_b                   8.506
_cell_length_c                   5.621
_cell_volume                     348.040
_citation_journal_id_ASTM        EJICFO
_cod_data_source_file            Munoz_EJICFO_2007_1387.cif
_cod_data_source_block           Fe0.92Ho1Mn1.08O4.74
_cod_original_cell_volume        348.0395
_cod_original_formula_sum        'Fe0.92 Ho1 Mn1.08 O4.74'
_cod_database_code               4031256
The structure of K3 Rh Cl6 (H2 O); a comparison of two independent X-ray structure determinations
Murray-Rust, P.; Murray-Rust, J.; Acta Crystallographica B (24,1968-38,1982) 31 (1975) 1037–1040; doi:

data_2106571
_publ_section_title
;
 The structure of K3 Rh Cl6 (H2 O); a comparison of two independent X-ray
 structure determinations
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              1037
_journal_page_last               1040
_journal_volume                  31
_journal_year                    1975
_chemical_formula_sum            'Cl6 H2 K3 O Rh'
_chemical_name_systematic        'K3 (Rh Cl6) (H2 O)'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.4
_cell_length_b                   15.65
_cell_length_c                   12.05
_cell_volume                     2338.423
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Murray-Rust_ACBCAR_1975_1948.cif
_cod_data_source_block           H2Cl6K3O1Rh1
_cod_depositor_comments
;
 Marking attached hydrogen atoms.

 Antanas Vaitkus,
 2017-03-24
;
_cod_original_formula_sum        'H2 Cl6 K3 O1 Rh1'
_cod_database_code               2106571
Crystal Structure and Spectra of Cesium Potassium Tetracyanonickelate(2-)
Musselman, R.L.; Stecher, L.C.; Watkins, S.; Inorganic Chemistry 19 (1980) 3400–3403; doi:

data_4343882
_publ_section_title
;
 Crystal Structure and Spectra of Cesium Potassium Tetracyanonickelate(2-)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3400
_journal_page_last               3403
_journal_volume                  19
_journal_year                    1980
_chemical_formula_sum            'C4 Cs K N4 Ni'
_chemical_name_systematic        'Cs K Ni (C N)4'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                60.64
_cell_angle_beta                 70.88
_cell_angle_gamma                70.88
_cell_formula_units_Z            2
_cell_length_a                   7.421
_cell_length_b                   8.626
_cell_length_c                   9.364
_cell_volume                     483.360
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Musselman_INOCAJ_1980_32.cif
_cod_data_source_block           C4Cs1K1N4Ni1
_cod_original_cell_volume        483.3596
_cod_original_formula_sum        'C4 Cs1 K1 N4 Ni1'
_cod_database_code               4343882
Study of metallic carbides by electron diffraction Part II. Crystal structure analysis of nickel carbide
Nagakura, S.; Journal of the Physical Society of Japan 13 (1958) 1005–1014; doi:

data_1528750
_publ_section_title
;
 Study of metallic carbides by electron diffraction Part II. Crystal
 structure analysis of nickel carbide
;
_journal_name_full               'Journal of the Physical Society of Japan'
_journal_page_first              1005
_journal_page_last               1014
_journal_volume                  13
_journal_year                    1958
_chemical_formula_sum            'C Ni3'
_chemical_name_systematic        'Ni3 C'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.553
_cell_length_b                   4.553
_cell_length_c                   12.92
_cell_volume                     231.947
_citation_journal_id_ASTM        JUPSAU
_cod_data_source_file            Nagakura_JUPSAU_1958_409.cif
_cod_data_source_block           C1Ni3
_cod_original_cell_volume        231.9468
_cod_original_formula_sum        'C1 Ni3'
_cod_database_code               1528750
Polysulfonylamine. CLVIII. Kristallstrukturen von Metall-di(methansulfonyl)amiden. 9. Erhoehung der Kristallsymmetrie durch Kokristallisation: Monoklines Na [(C H3 S O2)2 N].H2 O und tetragonales Na K [(C H3 S O2)2 N]2.2H2 O
Nagel, K.H.; Naeveke, M.; Blaschette, A.; Lange, I.; Moers, O.; Jones, P.G.; Zeitschrift fuer Anorganische und Allgemeine Chemie 628 (2002) 2877–2886; doi:

data_1528751
_publ_section_title
;
 Polysulfonylamine. CLVIII. Kristallstrukturen von
 Metall-di(methansulfonyl)amiden. 9. Erhoehung der Kristallsymmetrie durch
 Kokristallisation: Monoklines Na [(C H3 S O2)2 N].H2 O und tetragonales
 Na K [(C H3 S O2)2 N]2.2H2 O
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              2877
_journal_page_last               2886
_journal_volume                  628
_journal_year                    2002
_chemical_formula_sum            'C2 H8 N Na O5 S2'
_chemical_name_systematic        'Na ((C H3 S O2)2 N) (H2 O)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.97
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   23.943
_cell_length_b                   9.284
_cell_length_c                   15.258
_cell_volume                     3226.201
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Nagel_ZAACAB_2002_1053.cif
_cod_data_source_block           C2H8N1Na1O5S2
_cod_original_formula_sum        'C2 H8 N1 Na1 O5 S2'
_cod_database_code               1528751
Polysulfonylamine. CLVIII. Kristallstrukturen von Metall-di(methansulfonyl)amiden. 9. Erhoehung der Kristallsymmetrie durch Kokristallisation: Monoklines Na [(C H3 S O2)2 N].H2 O und tetragonales Na K [(C H3 S O2)2 N]2.2H2 O
Nagel, K.H.; Naeveke, M.; Moers, O.; Lange, I.; Jones, P.G.; Blaschette, A.; Zeitschrift fuer Anorganische und Allgemeine Chemie 628 (2002) 2877–2886; doi:

data_1528752
_publ_section_title
;
 Polysulfonylamine. CLVIII. Kristallstrukturen von
 Metall-di(methansulfonyl)amiden. 9. Erhoehung der Kristallsymmetrie durch
 Kokristallisation: Monoklines Na [(C H3 S O2)2 N].H2 O und tetragonales
 Na K [(C H3 S O2)2 N]2.2H2 O
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              2877
_journal_page_last               2886
_journal_volume                  628
_journal_year                    2002
_chemical_formula_sum            'C4 H16 K N2 Na O10 S4'
_chemical_name_systematic        'Na K ((C H3 S O2)2 N)2 (H2 O)2'
_space_group_IT_number           96
_symmetry_space_group_name_Hall  'P 4nw 2abw'
_symmetry_space_group_name_H-M   'P 43 21 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.696
_cell_length_b                   10.696
_cell_length_c                   28.741
_cell_volume                     3288.097
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Nagel_ZAACAB_2002_1054.cif
_cod_data_source_block           C4H16K1N2Na1O10S4
_cod_original_formula_sum        'C4 H16 K1 N2 Na1 O10 S4'
_cod_database_code               1528752
On the structure of staurolite, H Fe2 Al9 Si4 O24
Naray-Szabo, I.; Sasvari, K.; Acta Crystallographica (1,1948-23,1967) 11 (1958) 862–865; doi:

data_2310641
_publ_section_title
;
 On the structure of staurolite, H Fe2 Al9 Si4 O24
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              862
_journal_page_last               865
_journal_volume                  11
_journal_year                    1958
_chemical_formula_sum            'Al9 Fe2 H O24 Si4'
_chemical_name_systematic        'H Fe2 Al9 Si4 O24'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.1
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.82
_cell_length_b                   16.51999
_cell_length_c                   5.63
_cell_volume                     727.318
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Naray-Szabo_ACCRA9_1958_277.cif
_cod_data_source_block           H1Al9Fe2O24Si4
_cod_original_cell_volume        727.3179
_cod_original_formula_sum        'H1 Al9 Fe2 O24 Si4'
_cod_database_code               2310641
The crystal and molecular structure of bis-biuret-zinc chloride
Nardelli, M.; Fava, G.; Giraldi, G.; Acta Crystallographica (1,1948-23,1967) 16 (1963) 343–352; doi:

data_2310642
_publ_section_title
;
 The crystal and molecular structure of bis-biuret-zinc chloride
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              343
_journal_page_last               352
_journal_volume                  16
_journal_year                    1963
_chemical_formula_sum            'C4 H10 Cl2 N6 O4 Zn'
_chemical_name_systematic        '(Zn (C2 H5 N3 O2)2) Cl2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 124.7
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.02
_cell_length_b                   7.26
_cell_length_c                   11.54
_cell_volume                     552.414
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Nardelli_ACCRA9_1963_1907.cif
_cod_data_source_block           C4H10Cl2N6O4Zn1
_cod_original_cell_volume        552.4141
_cod_original_formula_sum        'C4 H10 Cl2 N6 O4 Zn1'
_cod_database_code               2310642